HHS Public Access Author manuscript Author Manuscript
Am J Dent. Author manuscript; available in PMC 2016 December 01. Published in final edited form as: Am J Dent. 2015 December ; 28(6): 357–361.
Depth of cure of bulk fill composites with monowave and polywave curing lights Timothy S. Meneesa, Chee Paul Lin, PhDb, Dave D. Kojic, DDS, MSc, John O. Burgess, DDS, MSa, and Nathaniel C. Lawson, DMD, PhDa,* aUniversity
of Alabama at Birmingham School of Dentistry, Clinical and Community Sciences, Department of Biomaterials, 1919 7th Avenue South, Birmingham, AL 35205
for Clinical and Translational Science, University of Alabama at Birmingham, 401P Medical Towers, 1717 11th Ave S, Birmingham, AL 35294 cUniversity
of Toronto School of Dentistry, Department of Restorative Dentistry, 124 Edwards St. Room 352, Toronto, Ontario M5G 1G6
Abstract Purpose—To measure and compare the depth of cure (DOC) of two bulk fill composite resins using a monowave and polywave light curing unit (LCU) according to ISO 4049 and using custom tooth molds.
Methods—The DOC of Tetric Evoceram Bulk Fill (Ivoclar Vivadent) and Filtek Bulk Fill Posterior (3M ESPE) were measured using a monowave LED LCU (Elipar S10 / 3M ESPE) and a polywave LED LCU (Bluephase G2 / Ivoclar Vivadent). Metal molds were used to fabricate 10 mm long DOC specimens (n=10) according to ISO 4049. Uncured composite material was scraped away with a plastic instrument and half the length of remaining composite was measured as the DOC. Custom tooth molds were fabricated by preparing >10mm long square-shaped (4 × 4 mm) holes into the mesial/distal surfaces of extracted human molars. Composite resin was placed into one end of the prepared tooth and light polymerized. Uncured composite resin was removed from the opposite side from which the tooth was irradiated and the tooth was sectioned mesiodistally. Half the length of remaining cured composite was measured as the DOC. Data were analyzed by three-way ANOVA (alpha=0.05) for factors material, LCU, and mold.
Results—The main effect LCU was not significant (p=.58). The interaction effect between material × mold was significant (p=.0001). The DOC of the composites differed significantly only with the stainless steel mold in which Tetric Evoceram Bulk Fill showed a deeper DOC than Filtek Bulk Fill Posterior (4.03 ± 0.14 vs 3.56 ± 0.38 mm, p10mm) was prepared by two trained operators under water lubrication using dental diamond burs (8856DF.31.016, Brasseler) in a high speed handpiece (Figure 1). The holes were examined with a periodontal probe to ensure dimensions were accurate to within 0.5 mm. If small perforations (less than 1 mm) occurred through the occlusal surface or pulp chamber, they were repaired with A3 resin composite (Z100, 3M ESPE). If a large perforation occurred, the tooth was discarded. An opaque adhesive strip was placed to cover one end of the hole (bottom), and the resin composite was then condensed into the other end of the hole (top). The LCU was centered over the top hole and positioned in contact with the composite material. Each composite was irradiated with both LCUs for the length of time recommended by the manufacturer. The adhesive strip was then removed, and the uncured resin composite was removed from the bottom hole. Using a diamond disc in a laboratory handpiece, the tooth was sectioned mesio-distally through the middle of the square-shaped hole into an occlusal and apical section (Figure 2). Any remaining uncured composite was scraped away with a plastic spatula. The maximum intact length of the RBC was measured with digital calipers to the nearest 0.01 mm and divided in half to determine DOC. Am J Dent. Author manuscript; available in PMC 2016 December 01.
Menees et al.
The DOC data were analyzed using a three-way ANOVA, followed by a post-hoc test for any significant factor or interaction. A p-value < 0.05 was considered statistically significant in two-tailed statistical tests. All analyses were conducted using SAS 9.4 (SAS Institute, Cary, NC, USA). The graphical displays were created by R 3.2.0. The mean irradiance (mW/cm2), total energy density (J/cm2), energy distribution per spectrum (J/cm2), and spectral irradiance (mW/cm2/nm) of each LED light was obtained by MARC® PS system (Blue Light Analytics). The MARC® device has built-in laboratory grade UV-VIS spectrometer (USB4000, Ocean Optics), spectral range from 365 – 515 nm and a laboratory-grade cosine-corrected sensor. This can measure intensity up to 10,000 mW/cm2 (integration times are used to enable changes in intensity and prevent saturation). The tested LCU light probe was set 0 mm from the sensor and the reading was rendered in 10 seconds utilizing MARC® software v. 3.04.
RESULTS Result of the three-way ANOVA is presented in Table 1. The DOC of two resin-based composites irradiated with two different LCUs in two different mold types are shown in Figure 3. The main effects of mold (p=.07) and LCU (p=.58) on DOC were not significant. Only the effect of material on DOC was significant (p=.007). However this effect was dependent on the mold and characterized by a significant interaction between the material and type of mold used (p=.0001). Using the stainless steel mold, Tetric Evoceram Bulk Fill produced a higher DOC compared to Filtek Bulk Fill Posterior (4.03 ± 0.14 vs 3.56 ± 0.38 mm, p